Colour degradation is a major problem in maxillofacial silicone elastomers. Recent studies have focused on colour stability and the mechanical properties of the silicone elastomers. A colour match is also essential for the acceptance of the prosthesis by the patient. The aim of this study is to assess the colour degradation of the silicone elastomer after being moulded in different colours of dental stones at two different vulcanization temperatures.
Five different colours of dental stones were used to fabricate a total of 120 silicone blocks using a Cosmesil M511 maxillofacial silicone elastomer. Vulcanization was completed at two different temperatures (25 and 100° Celsius). Colour measurements were obtained with a Conica Minolta spectrophotometer. The CIEDE2000 formula was used to calculate the colour differences (∆E00). Two-way ANOVA, one-way ANOVA with Bonferroni corrected post-hoc p values and independent samples t-test were used for the statistical analyses.
High temperature vulcanization causes lightening of the maxillofacial silicone elastomers without regard to the dental stone colour (p = 0.001). Specimens moulded in green stone lightened least at room temperature (p = 0.999). Compared to the control group, at high temperature, all specimens moulded in coloured dental stones darkened significantly (p < 0.001 for white, blue and yellow; p = 0.006 for green; p = 0.045 for reddish-brown). In the high temperature group, the shift to a green chroma was significant in the white, yellow and green dental stones groups (p = 0.001, p = 0.002, p < 0.001, respectively). The mean b* of the high temperature control group was higher than that of the room temperature control group (p < 0.001). The only ∆E00 score lower than the perceptibility threshold for dental materials (∆E00 = 1.30) was between the room temperature control group and the room temperature green dental stone group (∆E00 = 0.96).
Green and blue dental stones cause less colour degradation in silicone elastomers. Reddish-brown dental stones cause the most colour degradation in silicone elastomers. At 100 °C, the colour of the silicone elastomer lightens and yellows even if the elastomer is vulcanized in a stainless steel mould. White, yellow and reddish-brown dental stones make the silicone elastomer appear more yellow even if the elastomer is vulcanized at room temperature.
Beumer J, Curtis TA, Marunick MT. Maxillofacial rehabilitation: prosthodontic and surgical considerations. St Louis: Ishiyaku EuroAmerica Inc; 1996.
Mitra A, Choudhary S, Garg H, H G J. Maxillofacial prosthetic materials- an inclination towards silicones. J Clin Diagn Res. 2014;8(12):08-13.
Guiotti AM, Goiato MC, Dos Santos DM, Vechiato-Filho AJ, Cunha BG, Paulini MB, Moreno A, de Almeida MT. Comparison of conventional and plant-extract disinfectant solutions on the hardness and color stability of a maxillofacial elastomer after artificial aging. J Prosthet Dent. 2016;115(4):501–8. CrossRefPubMed
Ellias HG, Mülhaupt R. Plastics, general survey, 1. definition, molecular structure and properties. In: Elvers B, editor. Ulmann’s polymers and plastics: products and process, vol. 1. Germany: Willey-VCH; 2016. p. 37–68.
Stein RS, Powers J. Topics in polymer physics. London: Imperial College Press; 2006. CrossRef
Kulkarni RS, Nagda SJ. Colour stability of maxillofacial silicone elastomers: a review of the literature. Eur J Prosthodont Restor Dent. 2014;22(3):108–15. PubMed
Akash RN, Guttal SS. Effect of Incorporation of Nano-Oxides on Color Stability of Maxillofacial Silicone Elastomer Subjected to Outdoor Weathering. J Prosthodont. 2015; doi: 10.1111/jopr.12252.
Han Y, Zhao Y, Xie C, Powers JM, Kiat-amnuay S. Color stability of pigmented maxillofacial silicone elastomer: effects of nano-oxides as opacifiers. J Dent. 2010;38(2):100–5. CrossRef
Kiat-amnuay S, Beerbower M, Powers JM, Paravina RD. Influence of pigments and opacifiers on color stability of silicone maxillofacial elastomer. J Dent. 2009;37(1):45–50. CrossRef
Kheur M, Sethi T, Coward T, Kakade D, Rajkumar M. Evaluation of the effect of ultraviolet stabilizers on the change in color of pigmented silicone elastomer: An in vitro study. J Indian Prosthodont Soc. 2016;16(3):276–81. PubMed
Ghinea R, Pérez MM, Herrera LJ, Rivas MJ, Yebra A, Paravina RD. Color difference thresholds in dental ceramics. J Dent. 2010;38(2):57–64. CrossRef
Rugh EH, Johnston WM, Hesse NS. The relationship between elastomer opacity, colorimeter beam size, and measured colorimetric response. Int J Prosthodont. 1991;4(6):569–76. PubMed
Johnston WM, Ma T, Kienle BH. Translucency parameter of colorants for maxillofacial prostheses. Int J Prosthodont. 1995;8(1):79–86. PubMed
Hu X, Johnston WM. Translucency estimation for thick pigmented maxillofacial elastomer. J Dent. 2011;39(1):2–8. CrossRef
Sharma G, Wu W, Dalal NE. The CIEDE2000 color-difference formula: implementation notes, suplementary test data, and mathematical observations. Color Res Appl. 2005;30:21–30. CrossRef
Griniari P, Polyzois G, Papadopoulos T. Color and structural changes of a maxillofacial elastomer: the effects of accelerated photoaging, disinfection and type of pigments. J Appl Biomater Funct Mater. 2015;13(2):87–91.
Lynch DK, Livingston W. Colour and light in nature. 2nd ed. Cambridge: Cambridge University Press; 2001.
Perroni AP, Amaral C, Kaizer MR, Moraes RR, Boscato N. Shade of resin-based luting agents and final color of porcelain veneers. Esthet Restor Dent. 2016;28(5):295–303. CrossRef
- Effect of vulcanization temperature and dental stone colour on colour degradation of maxillofacial silicone elastomers
Ebru Demet Cifter
Meltem Ozdemir – Karatas
- BioMed Central
Neu im Fachgebiet Zahnmedizin
Mail Icon II